**4. Defect stability – formation energy and concentration 34**

**6.1. Neutral oxygen vacancy in bulk MgO**

**6. F centers in bulk MgO**

MgO crystallizes in the rock-salt structure, where each atom is six-fold coordinated in the bulk (Fig.6.1). The experimentally determined lattice constant for MgO is 4.207 Å atT = 0 K[177].

When the effects of zero-point vibrations are removed, the lattice constant is 4.186 Å [178]. The bonding type in MgO is strongly ionic, with formal ion charges of magnesium and oxygen 2+

and 2-, respectively. Although the experimental bandgap of MgO is 7.78 eV, as measured by reflectance spectroscopy [179], realistic samples are typically neither clear transparent nor in-sulating. Defects such as intrinsic point defects, impurities and defect complexes are not only responsible for the color of the samples, but can also give rise to electron or hole conductiv-ity [32,180,181].

**Figure 6.1.: Simple cubic unit cell of MgO.**

Oxygen vacancies are typically studied in the context of their influence on the oxide
proper-ties. These point defects are also called color centers or F centers, referring to the German word
*Farbzentrum, due to their effect on the optical properties. Despite numerous studies, the *
ac-tual abundance of oxygen vacancies at realistic conditions remains undetermined. Even for the
simplest type of oxygen vacancy, the neutral F^{0} center in MgO bulk, the challenge to obtain an
accurate estimate for point defect formation energies in experiment and theory becomes evident,
since reported experimental and theoretical results disagree severely. In the following, electronic
and geometric structure of bulk F centers in MgO are studied, and formation energies as well
as electronic levels are tested for their dependence on DFT exchange-correlation treatment. The
goal is to find a reliable exchange-correlation functional for the analysis of neutral and charged
F centers in MgO.

6.1. Neutral oxygen vacancy in bulk MgO following paragraphs, using periodic and embedded cluster models and comparing DFT and hybrid DFT results to high level coupled-cluster theory values.

**Experimentally measured formation energy**

In Kappers’ experiment the bulk oxygen vacancies are created by additive coloring [26]. Single
crystals of MgO are heated in magnesium vapor at temperatures from 1,870 K to 2,100 K under
pressures up to 5.3 atm. The high magnesium chemical potential lowers the formation energy
of the bulk F centers (compare Eq.4.1and Eq.4.11) and allows for them to form in detectable
concentration. Optical absorption experiments are then performed, and from the maximum
in-tensityu_{max}and width at half-maximumU of the absorption peak the density of F^{0}centersn_{F}^{0}
can be obtained. For this, the Gaussian form of the Smakula formula [182] is used, depending
also on oscillator strengthf_{os} (a measure of the transition strength) and the index of refraction
k:

n_{F}^{0} ∝ k
(k^{2}+ 2)^{2}

1 fos

u_{max}U. (6.1)

The ratio between F^{0} center density and the density of atoms in the magnesium vapor is
shown in Fig.6.2*(left) for several crystals colored at 2,086 K and 1,885 K. In thermodynamic*
equilibrium, the increase in free energy if one atom is removed from the magnesium vapor is
equal to the increase in free energy if one magnesium atom is added to the crystal and a bulk F
center is formed. This relates the ratio of the density of F^{0} centers and the magnesium atoms in
the vapor to the defect formation enthalpy∆H_{f} atT = 0 Kwith respect to cohesive energy of
the MgO crystal via

n_{F}^{0}/nMg = C·e^{−}

∆Hf kBT

. (6.2)

∆H_{f}is the enthalpy change upon removal of a neutral oxygen atom from MgO bulk and placing
it into the gas phase. The cohesive energy is defined as the energy cost of separating an MgO
crystal into free magnesium and oxygen atoms, per Mg-O pair. The dependence of C on
tem-perature is weak, and is therefore neglected. From the density ratio, measured as a function of
temperature,∆H_{f}can thus be obtained by a fit to Eq.6.2, as shown in Fig.6.2*(right).*

The experimental value for the F^{0}formation enthalpy estimate atT = 0 Kis 1.53 eV above
the cohesive energy with respect to oxygen atom (µ_{O} = E_{O}), and -1.06 eV with respect to O_{2}
molecule (µ_{O} = 1/2E_{O}2). Adding the experimental cohesive energy of 10.35 eV [183] results
in a formation enthalpy of 11.88 eV with respect to oxygen atom, or 9.29 eV with respect to O2

molecule.

As also mentioned by Kappers [26], it is hard to ensure that thermal equilibrium is reached when the crystals are colored. Additional uncertainty enters through assumptions made to de-rive Eq.6.1, which may be problematic for ionic solids, as pointed out by Dexter [182]. Also specifics of the estimate made for the oscillator strength are not documented. Therefore, com-parison with different experiments would be desirable.

6.1. Neutral oxygen vacancy in bulk MgO

**Figure 6.2.: Left: Equilibrium density of F**^{0}centersn_{F}^{0} as a function of the density of atoms in
the magnesium vaporn_{Mg}*Right: Ratio of the density of F*^{0}centers to the density of atoms in the
vapor as a function of the reciprocal temperature. Each filled point, except for the one measured
at an intermediate temperature, corresponds to one data point in the graph on the left. The two
open points in the right graph correspond to the two linear fits in the graph on the left. Graphs
are taken from Ref. [26], labels have been adjusted to match denotations in the text. (Copyright
(1970) by The American Physical Society.)

**Theoretical results**

The formation energy for the F^{0}center has been calculated and reported in literature using
dif-ferent methods and models [27–30]. Fig.6.3 summarizes these results, comparing formation
energies G^{0}_{f}(T = 0, p^{0})according to Eq. 4.1 in the oxygen-rich limit (µ_{O} = 1/2E_{O}^{tot}_{2}). The
zero-point vibrational energy contribution to the formation energy, estimated using the
finite-displacement method for a2×2×2MgO bulk unit cell, is -0.12 eV. Vibrational energy
contri-butions are neglected in the following. It becomes evident that the experimental estimate for the
F^{0} center formation energy of 9.29 eV is in disagreement with the results reported in literature
and with the formation energies calculated within this work (red symbols in Fig.6.3).
Forma-tion energies calculated with LDA are surprisingly closest to the experimental estimate. LDA
is known to systematically overestimate the binding between atoms in crystals [184], hence a
higher formation energy is obtained than for the other methods used. Compared to the
experi-mental MgO lattice constant of 4.186Å [177,178] (extrapolated toT = 0 K), the lattice constant
optimized with LDA underestimates (4.165 Å), while PBE (4.258 Å), HSE06 (4.218 Å) and
PBE0 (4.212 Å) optimized lattice constants overestimate. For details on lattice parameter
op-timization see appendix A.3. Geometric relaxation effects play a minor role for formation of
F^{0} centers. The relaxation energy due to the removal of oxygen is 0.1 eV at PBE level, and
therefore only makes up for 1.4% of the formation energy (7.09 eV). Already for a2×2×2
supercell, containing 64 atoms, the formation energy of the neutral oxygen vacancy is converged
with respect to the supercell size. The two defect electrons remain localized at the vacancy site.

6.1. Neutral oxygen vacancy in bulk MgO They occupy a defect level in the middle of the bandgap, and are therefore higher in energy than the electrons associated with the regular ionic bonding in the MgO lattice (see also Fig.6.10).

LDA GGA HSE ω=0.5

HSE06 PBE0 B3LYP HF HF+MP2 5.5

6 6.5 7 7.5 8 8.5 9

Formation energy (eV)

periodic cluster

**Figure 6.3.: F**^{0} center formation energy in the oxygen-rich limit (µ_{O} = 1/2E_{O}^{tot}_{2}). Literature
results forµ_{O}=E_{O}^{tot} were recalculated forµ_{O} = 1/2E_{O}^{tot}_{2} using the experimental O_{2}binding
energy. Different types of exchange-correlation treatment and periodic (circles) or embedded
cluster (triangles) models were used. Red circles show results obtained within this work, orange
triangles were calculated in a collaboration by S. Sicolo [185]. From literature, periodic DFT
calculations at LDA level (blue circle, [27]; green circle [28]) and GGA level (green circle,
PBE [28]; gray circle, PW91 [29]), as well as embedded cluster calculations applying HF and
HF+MP2 (black triangles [30]) are shown for comparison.

The results calculated with periodic models using the HSE family of functionals, including
PBE and PBE0, agree within 0.15 eV, if the O_{2}binding energy is corrected, but are≈2 eV lower
than the experimental result. The experimental estimate was originally obtained with respect to
cohesive energy. Therefore, to compare directly with the measured quantity, G^{0}_{f} is calculated
with respect to cohesive energy

E_{MgO}^{coh} =E_{MgO}^{bulk} −E_{Mg}^{tot} −1/2E_{O}^{tot}_{2}, (6.3)
whereE_{MgO}^{bulk} is the total energy of bulk MgO per MgO unit, E_{Mg}^{tot} is the total energy of a Mg
atom, and the total energy of oxygenE_{O}^{tot}_{2} is obtained using the experimental binding energy, as
described in Sec.4.1.2, for different parameter sets (α, ω) (Fig.6.4). However, the discrepancy
between experiment and theory is still mainly due to the formation energy, not the cohesive
energy.

*It was demonstrated by Ramprasad et al. in 2012 that there is a near-linear correlation between*
the formation energies of neutral point defects in bulk Si, Ge, ZnO, and ZrO_{2} and the
corre-sponding valence bandwidth (VBW) of the defect-free parent material, when both are computed
as a function of the HSE parameters [186]. The deviations from linearity increase when the
bandgap is used instead of the VBW. The bandgap was already pointed out to be an unreliable
descriptor for defect formation energies by Lany and Zunger in 2010 [187]. The prescription for
*finding reliable formation energies for neutral point defects suggested by Ramprasad et al. is to*
find a DFT functional that gives the experimental VBW for the given material – which requires
only pristine bulk calculations –, and use the corresponding exchange-correlation functional to
compute the accurate defect formation energies.

6.1. Neutral oxygen vacancy in bulk MgO

**Figure 6.4.: F**^{0}center formation energy with respect to cohesive energy (Eq.6.3) in the
oxygen-rich limit^{1}, calculated for different parameter sets (α,ω) of the HSE hybrid-functional family.

Formation energies are shown as a function of oxygen 2pbandwidth, the solid red line indicates the experimental value [26].

For MgO, the bulk neutral F center formation energyG^{0}_{f} only weakly depends on the exchange
and screening parameters of HSE. Still, a near-linear correlation with small but finite slope is
found for G^{0}_{f} as a function of oxygen 2 p bandwidth (Fig. 6.5). However, the methodology
suggested in Ref. [186] cannot be applied to MgO, because of a large uncertainty in experimental
oxygen 2pbandwidth [188–191].

**Figure 6.5.: F**^{0} center formation energy, calculated for different parameter sets of HSE(α, ω)
(black symbols), shown as a function of oxygen 2pbandwidth (black line shows linear fit). The
red line indicates the experimentally measured formation energy [26]. The blue lines depict
ex-perimental values for the MgO oxygen 2pbandwidth, measured using electron momentum
spec-troscopy (EMS) [191], angle-resolved ultraviolet photoelectron specspec-troscopy (APRES) [190],
x-ray photoelectron spectroscopy (XPS) [189] and x-ray emission spectroscopy (XES) [188].

*Another approach is to benchmark HSE functionals against higher-level ab initio methods,*

1In this work, the oxygen-rich limit is always calculated using the experimental O2binding energy as described in Sec.4.1.2

6.1. Neutral oxygen vacancy in bulk MgO

**Figure 6.6.: Formation energy of the neutral oxygen vacancy at the center of a) an **
unembed-ded Mg6O1 (with a charge +10) and b) an unembedded Mg14O13 (with a charge +2) cluster
model, calculated at different levels of electronic structure theory using NWChem (red squares)
*with basis sets up to cc-pVTZ, and FHI-aims (blue triangles) with basis sets up to tight, tier 4.*

Formation energies have been corrected for the basis set superposition error using the
counter-poise correction method (see Appendix A.4for details). In the NWChem calculations for the
Mg_{14}O_{13} cluster, only the cc-pVDZ basis set could be used for the∆MP2 and∆CCSD
cor-rections [192–195], since employing a higher-level basis set (cc-pVTZ) using these methods in
the available implementation was computationally not feasible due to extremely high memory
consumption.

such as coupled-cluster theory with single and double excitations (CCSD), CCSD plus triple
excitations by perturbation theory (CCSD(T)), RPA orGW. This can be performed efficiently
using cluster models. First, two MgO clusters are calculated: a six-coordinated oxygen atom
(Mg6O1), and a 27-atom MgO cube (Mg14O13) (see Fig.6.6). The clusters were constructed
using the PBE optimized lattice constant of bulk systems. In both clusters there are more
mag-nesium atoms than oxygen atoms. The clusters are therefore charged by removing all magmag-nesium
valence electrons that cannot be accommodated by oxygen atoms (counting two electrons per
oxygen atom). This corresponds to a charge +10 for Mg_{6}O_{1} and a charge +2 for Mg_{14}O_{13}.
The oxygen removal energies for these two (unrelaxed) systems are calculated at different levels

6.1. Neutral oxygen vacancy in bulk MgO
of electronic structure theory, where possible using two different all-electron codes, FHI-aims
and NWChem. Since the cluster models are not embedded, the oxygen removal energies are
not quantitatively comparable to those of the F^{0} center in extended material. However, for each
cluster model, the formation energy of the neutral F center calculated with CCSD is close to the
results obtained with PBE (α = 0, ω = arbitrary) and PBE0 (α= 0.25, ω = 0). The formation
energies obtained with CCSD are much closer to the HSE results than to the experimental value.

This result has been corroborated in a cooperation with Prof. Sauer’s theoretical chemistry
group of the Humboldt-Universität zu Berlin. Embedded cluster calculations at PBE, PBE0 and
B3LYP level and with the CCSD(T) coupled-cluster method were performed using the
TURBO-MOLE code [96]. For the DFT TURBOTURBO-MOLE calculations on embedded clusters, [5s3p2d1f] /
[5s4p3d] triple-zeta valence plus polarization basis sets were used [196]. For the CCSD(T)
com-putations also electrons in the magnesium 2sand 2pshells were correlated using core-valence
correlation consistent basis sets, cc-pCVXZ (X = D, T, Q) for magnesium, whereas on the O^{2−}

ions the aug-cc-pVXZ basis sets were used [197]. For consistency between FHI-aims and
TUR-BOMOLE, embedded cluster calculations at PBE, PBE0 and B3LYP level were also performed
with FHI-aims using the same cluster models. In both CCSD(T) and DFT calculations, the
basis set superposition error (BSSE) was evaluated following the Boys-Bernardi counterpoise
correction [198]. The MgO clusters are embedded in a periodic point charge array using the
pe-riodic electrostatic embedded cluster model [199] in TURBOMOLE, and a converged finite set
of point charges in FHI-aims. To minimize non-physical polarization of peripheral oxygen
an-ions by the embedding point charges, pseudopotentials are added to the first shell of embedding
Mg^{2+}cations (all-electron Hay&Wadt effective core potentials (ECPs) [200] in TURBOMOLE,
and Troullier-Martins-type norm-conserving non-local pseudopotentials [201,202] in FHI-aims
calculations). The PBE lattice constant is used for the embedded clusters. Apart from the
outer-most frozen shell of atoms, full relaxation is allowed in the DFT calculations for larger clusters
(Mg_{14}O_{19}). For the CCSD(T) calculations and respective DFT values obtained for smaller
clus-ters (Mg_{6}O_{9}), formation energies of neutral, unrelaxed F centers are compared.

G^{0}_{f} is calculated at very high accuracy with CCSD(T) for the embedded Mg_{6}O_{9} cluster
(Fig. 6.7), the largest model that is still computationally feasible, due to high memory
con-sumption. The CCSD(T) value is compared to the formation energies calculated for the same
system with various DFT functionals, yielding a correction term∆CCSD(T) for each DFT
func-tional. The correction term is finally added to the DFT formation energies calculated for a larger
cluster Mg_{14}O_{19}that is converged also with respect to geometric relaxation.

Table6.1summarizes the formation energies for a neutral F^{0} center in MgO bulk calculated
with the Mg_{6}O_{9}model, and formation energies including geometric relaxation as obtained with
an Mg_{14}O_{19}embedded cluster. For consistency, formation energies calculated with FHI-aims
*for the same cluster models using a tight, tier 3 basis, and for periodic models using a tight,*
tier 2 basis are also shown. Obviously, the formation energy of the unrelaxed defect is already
converged within 0.1 eV with respect to cluster size.

The corrections∆CCSD(T) for the DFT formation energies are−0.09eV for PBE,0.07eV
for PBE0, and −0.28eV for B3LYP. Adding these corrections to the DFT formation energies
obtained with a converged cluster size Mg_{14}O_{19} (with charge -10), yields DFT+∆CCSD(T)
results of 6.85 eV, 6.88 eV, and 6.89 eV, respectively.

From this it is concluded that the formation energies for neutral F centers can be calculated

6.1. Neutral oxygen vacancy in bulk MgO

**Figure 6.7.: Mg**_{6}O_{9} cluster model (with charge -6), embedded by magnesium core potentials.

Embedding point charges (see text) are not shown. CCSD(T) calculations were performed using
this model at unrelaxed bulk F^{0} geometry, where the central oxygen atom in the cluster was
removed.

**Table 6.1.: Formation energies,**G^{0}_{f}, calculated for unrelaxed (unrel.) and relaxed (rel.) atomic
coordinates for a bulk F^{0}center, as obtained from embedded cluster DFT and CCSD(T)
calcu-lations employing FHI-aims (AIMS) and the TURBOMOLE (TURB.) code.

Structure model PBE HSE06 PBE0 B3LYP RPA rPT2 CCSD CCSD(T)

@PBE @PBE

Mg_{6}O_{9}(unrel.,TURB.) 7.18 – 7.02 7.37 – – 7.05 7.09

Mg_{6}O_{9}(unrel.,AIMS) 7.11 7.03 6.99 7.35 7.13 7.45 – –

Mg_{14}O_{19}(unrel.,TURB.) 7.06 – – – – – – –

Mg_{14}O_{19}(rel.,TURB.) 6.94 – 6.81 7.17 – – – –

Mg_{14}O_{19}(rel.,AIMS) – 7.05 – – – – – –

periodic (rel.,AIMS) 7.09 7.04 7.07 – – – – –

accurately to within 0.2 eV even at PBE level. In particular, the DFT+∆CCSD(T) formation
en-ergy values are in good agreement with the HSE06 F^{0} formation energies 7.04 eV and 7.05 eV,
obtained from the Mg14O19embedded cluster and periodic calculations, respectively, using
FHI-aims. It is concluded that the experimental value for the bulk F^{0} center formation enthalpy in
MgO [26] is a significant overestimate. The most likely reason is that thermodynamic
equilib-rium was not reached in the experiment.

Based on the accurate value of the formation energy, the reasons for the failure of certain electronic structure methods to accurately describe the removal of a neutral oxygen atom from MgO bulk can be deduced (see Fig.6.3 and Fig. 6.6): using the local density approximation leads to overestimated formation energies, while not including electron correlation yields

un-6.2. Charged defects in bulk MgO